10182

# Matrix Transformations in Crystallography

This Demonstration shows how various symmetry operations are used to simplify matrices; this process is called the direct inspection method. Select a crystallographic point group, the dimension of the matrix representation (number of rows × number of columns), and whether the original matrix should be assumed symmetric (only square matrices can be symmetric). The top row is the original untransformed matrix and the next row down displays the symmetry operations needed for the selected point group with the associated transformation matrix. The bottom row shows the result of each successive transformation step from left to right. It is in the last row that the matrix is progressively simplified, thus reducing the number of independent matrix elements.

### DETAILS

The symmetry operations used in this Demonstration correspond to the symmetries of the 32 crystallographic point groups. Each element in the matrix corresponds to a material parameter for a crystal. The matrix dimensions correspond to common electrical, mechanical, magnetic, and optical interactions in crystalline materials; for example, 3×3 matrices are used to represent permittivity or the refractive index, 3×6 matrices correspond to the piezoelectric effect, and 6×3 matrixes correspond to the linear electro-optic effect. The same is true for 6×6 matrices; for these the matrix can be assumed to be symmetric (e.g. the element in row , column is the same as the one in row , column ), which is the case for elastic stiffness. A nonsymmetric 6×6 matrix would include the elasto-optic effect, electrostriction, and magnetostriction. The resulting matrices and method of derivation are nicely explained in [1].
There are a few situations where this Demonstration may disagree with conventions used in some books. For example, the 6×3 point group 4 uses the coefficient though could also be used; this is because and are equal, so the choice of one over the other is arbitrary. The transformations agree with those given in [1]. The matrices are transformed with and directional cosine matrices as follows:
,
,
,
.
Reference
[1] R. E. Newnham, Properties of Materials, New York: Oxford University Press, 2005.

### PERMANENT CITATION

 Share: Embed Interactive Demonstration New! Just copy and paste this snippet of JavaScript code into your website or blog to put the live Demonstration on your site. More details » Download Demonstration as CDF » Download Author Code »(preview ») Files require Wolfram CDF Player or Mathematica.

#### Related Topics

 RELATED RESOURCES
 The #1 tool for creating Demonstrations and anything technical. Explore anything with the first computational knowledge engine. The web's most extensive mathematics resource. An app for every course—right in the palm of your hand. Read our views on math,science, and technology. The format that makes Demonstrations (and any information) easy to share and interact with. Programs & resources for educators, schools & students. Join the initiative for modernizing math education. Walk through homework problems one step at a time, with hints to help along the way. Unlimited random practice problems and answers with built-in Step-by-step solutions. Practice online or make a printable study sheet. Knowledge-based programming for everyone.